Raman enhancement by graphene-Ga2O3 2D bilayer film
© Zhu et al.; licensee Springer. 2014
Received: 23 December 2013
Accepted: 19 January 2014
Published: 28 January 2014
2D β-Ga2O3 flakes on a continuous 2D graphene film were prepared by a one-step chemical vapor deposition on liquid gallium surface. The composite was characterized by optical microscopy, scanning electron microscopy, Raman spectroscopy, energy dispersive spectroscopy, and X-ray photoelectron spectroscopy (XPS). The experimental results indicate that Ga2O3 flakes grew on the surface of graphene film during the cooling process. In particular, tenfold enhancement of graphene Raman scattering signal was detected on Ga2O3 flakes, and XPS indicates the C-O bonding between graphene and Ga2O3. The mechanism of Raman enhancement was discussed. The 2D Ga2O3-2D graphene structure may possess potential applications.
61.46.-w (structure of nanoscale materials), 68.65.Pq (graphene films), 74.25.nd (Raman and optical spectroscopy)
KeywordsGraphene Raman enhancement Gallium oxide Chemical vapor deposition
The assembly of graphene with other nanostructures can broaden the graphene applications. Considerable investigation has been carried out on the assembly of graphene powder with functional materials, such as reduced graphene oxide-TiO2 composites to enhance photocatalytic degradation activity [1–3], graphene-MoS2 for high effective hydrogen evolution reaction [4, 5], and graphene-Co3O4/Fe3O4 as anode material for lithium ion battery [6–9]. Two typical approaches for the assembly are extensively used. One is the hydrothermal approach wherein graphene oxide powder and other precursors are mixed with water or organic solvents and then undergo a hydrothermal process [1–5, 7]. The other approach is the mixing of reduced graphene oxide with the other materials followed by post-thermal reduction [6, 8, 9]. In addition, the assembly of functional materials on continuous graphene films synthesized by chemical vapor deposition (CVD) has been attracting attention gradually, owing to the high quality of graphene films. For example, a thin amorphous aluminum oxide layer was deposited on a graphene film through atomic layer deposition to selectively decorate and passivate the edges of graphene nanoribbons . ZnO was also deposited on CVD graphene, and the composite could be applied to a solar cell to replace ITO . A graphene/single-wall carbon nanotube hybrid was synthesized by a facile catalytic CVD growth on layered double hydroxide at high temperature, and the hybrid structure exhibited excellent performance in Li-S batteries with a high capacity .
Ga2O3 is a deep ultraviolet transparent semiconductor [13, 14], which has several different crystalline phases, including α-, β-, γ-, δ-, and ϵ-Ga2O3. Among these phases, monoclinic structured β-Ga2O3 is the most stable form with a wide bandgap of 4.9 eV . Because of its good luminescence properties, β-Ga2O3 has a useful application in phosphors. The hybrid structure of graphene and Ga2O3 is promising for flexible display devices by exploiting high conductivity and flexibility of graphene and the good luminescence of Ga2O3. Herein, we report a simple and one-step CVD process to assemble β-Ga2O3 flakes on a continuous graphene film. The morphology of the composite was characterized by optical microscopy (OM), field emission scanning electron microscopy (FESEM), Raman spectroscopy, and energy dispersive spectroscopy (EDS) mapping. The assembly mechanism was discussed. Importantly, it was found that the as-grown β-Ga2O3 flakes enhanced the intensity of the graphene Raman signal ten times. The possible Raman enhancement mechanism is proposed.
A 0.2 g Ga with 7 N purity from UMC was laid on a designed quartz bowl, loaded into the quartz tube, and heated to 1,000°C under the protection of 200 sccm Ar and 2 sccm H2. The sample was annealed at 1,000°C for 1 h to remove the surface oxide. The graphene film was synthesized through CVD for only 3 min under 200 sccm Ar flow with 1.5 sccm CH4. After the growth of the graphene, the carbon source was turned off and the temperature was kept at 1,000°C for 30 min. Then, the furnace cover was opened for fast cooling down to room temperature either immediately at 1,000°C or after controllably cooling (approximately 10°C/min) down first to 800°C, 600°C, and 400°C, respectively. The samples were placed in a refrigerator for several hours for solidification before characterization since the melting temperature of gallium is about 29.8°C and has strong supercooling effects, causing its liquid state at room temperature.
OM (Leica Microscopy DM6000M, Germany) was used for the preliminary exploration. Raman microprobe spectroscopy (Thermo Fisher DXR, Waltham, MA, USA) with an Ar+ laser (excitation wavelength 532 nm, 1 to 5 mW, and beam spot approximately 1 μm), FESEM (FEI NOVA NanoSEM with an operating voltage of 5 kV, Hillsboro, OR, USA), and energy dispersive spectroscopy (EDS) analysis (Oxford X-max 80, Oxfordshire, UK) were employed to characterize the samples. X-ray photoelectron spectroscopy (XPS, Thermo Scientific ESCALAB 250) with a monochromatized Al Kα X-ray source (1,486.6 eV photons) was used to study the bonding between graphene and Ga2O3. A Shirley background was removed from the atomic spectra prior to deconvolution. We tried to conduct an atomic force microscopy and transmission electrical microscopy in order to directly characterize the thickness and the interface between the layers, but the graphene film decorated by Ga2O3 flakes curled up after removing the Ga substrate, rendering high-quality sample impossible.
Results and discussion
The surface-enhanced Raman scattering (SERS) has been extensively investigated [18–20]. The charge transfer between the two contacted materials is the chemical mechanism of Raman enhancement [21, 22]. For the graphene Raman enhancement by β-Ga2O3 flakes, the charge transfer is confirmed by the Raman and XPS data. In the Raman spectra of Figure 2a and Additional file 1: Figure S1, the G-band has a downshift of approximately 2 cm−1 (1,584 to 1,582 cm−1) at the locations of the β-Ga2O3 sheets, which indicates the charge transfer between the graphene and β-Ga2O3, and β-Ga2O3 as an electron donor to the graphene . In addition, the work function of graphene (4.2 eV)  and Ga2O3 (4.11 ± 0.05 eV)  is proximity; this is consistent with the slight downshift of the graphene G-band. In addition to the Raman data, the XPS data also support the CM mechanism. Additional file 1: Figure S3 shows the XPS spectrum, showing a general scan in the energy range from 0 to 1,200 eV. The peaks of the core levels of Ga2p, Ga3s, Ga3p, Ga3d, and Ga LMM peaks, as well as the O1s, OKLL, and C1s, were detected. Additional file 1: Figure S4 shows the O1s peak with a binding energy around 532 eV, which is corresponds to the Ga-O bonding of Ga2O3. The two peaks of Ga2p for the Ga-O bondings are also clearly observed in Figure 4c [26, 27]. A high-resolution XPS C1s spectrum is given in Figure 4d. Using a suitable application of Gaussian and Lorentzian functions, the C1s peak can be decomposed into three apparent spectral components at 284.7, 285.7, and 286.2 eV. The main peak at 284.7 eV corresponds to the graphite-like sp2 C, and the 285.7 and 286.2 eV peaks are attributed to sp3 carbon and C-O bonds [24, 28]. The XPS data is consistent with the aforementioned Raman and EDS results to confirm the Ga2O3-graphene structure, and XPS also presents the evidence of the C-O bands, which confirms the negative-charge doping effect from the Ga2O3 sheets on the graphene film. Due to chemical doping, polarizability of graphene is increased, leading to an increase in the Raman scattering cross-section .
It is necessary to discuss the formation mechanism of Ga2O3-graphene. Ga itself is very reactive and can react with most materials under high temperature. In the periodic table of elements, Ga and Al are in the same main group and have similar characteristics. Analogously, Ga can form a continuous and compact oxidized layer in air, which impedes further oxidation of Ga. Therefore, we need to remove the very thin surface oxide before graphene growth through pre-annealing in Ar/H2 atmosphere. During the CVD graphene growth, hydrogen is hazardous for the graphene formation , and H2 was not applied during the growth stage. We proposed that the graphene grows on the surface of the liquid Ga at first and then the Ga2O3 sheets come into being on the graphene during the cooling process, as shown in the schematic illustration of Additional file 1: Figure S4. The O element comes from the oxygen residue in the tube, and the C-O bonds which have been evidenced by XPS are the defects on the 2D graphene film. These defects play an important role for the growth of Ga2O3 on graphene because they will act as nucleation points of Ga2O3 since Ga atoms in the vapor will obviously prefer O as a bonding target, not the carbon atoms.
This mechanism is supported by two evidences. The first one is that after immersing the samples of 2D Ga2O3-2D graphene into dilute hydrochloric acid for 1 h at room temperature, the Ga2O3 sheets will disappear. If the graphene covers and protects the Ga2O3 sheets, it is hard to remove Ga2O3 in hydrochloric acid. Another evidence is related to the cooling process. We chose different rapid cooling starting points of 800°C, 600°C, and 400°C. More polygon sheets or granules deposited on the graphene surface when the sample underwent longer cooling durations. According to the illustration depicted in Additional file 1: Figure S4, it is possible to control the deposition of Ga2O3 sheets on the graphene surface to form the special 2D Ga2O3 nanosheet-2D graphene sheet structure through a one-step CVD process. Compared to the general Raman enhancement by metals, such as silver and gold, the Ga2O3 nanosheets have remarkable thermal stability. Conversely, silver will oxidize excessively and becomes quenched within 36 h in the air . The 2D graphene-Ga2O3 film can be transferred onto other targets and may be used as bio-substrate through SERS. The stability of the Ga2O3 nanosheets and the structure stability need to be further investigated.
In summary, separated 2D thin Ga2O3 nanosheets, with a lateral size of 1 to 10 μm, on continuous 2D graphene film were synthesized by a one-step CVD process on liquid gallium substrate. The Raman and EDS mapping confirm the formation of the β-Ga2O3 sheets on the graphene surface. The formation mechanism was proposed as a β-Ga2O3 sheet formation after graphene synthesis during the cooling process. The graphene Raman enhancement over ten times was detected on the β-Ga2O3 sheets due to the charge transfer. The 2D-2D structure may have potential application in optical and electronic devices.
This work was supported by projects from the National Science and Technology Major Project (Grant No. 2011ZX02707), the National Natural Science Foundation of China (Grant No. 11104303, 11274333, 11204339 and 61136005) and Chinese Academy of Sciences (Grant No. KGZD-EW-303, XDA02040000 and XDB04010500).
- Wang WS, Wang DH, Qu WG, Lu LQ, Xu AW: Large ultrathin anatase TiO2 nanosheets with exposed 001 facets on graphene for enhanced visible light photocatalytic activity. J Phys Chem C 2012, 116: 19893–19901. 10.1021/jp306498bView ArticleGoogle Scholar
- Pastrana-Martínez LM, Morales-Torres S, Likodimos V, Figueiredo JL, Faria JL, Falaras PP, Silva AMT: Advanced nanostructured photocatalysts based on reduced graphene oxide–TiO2 composites for degradation of diphenhydramine pharmaceutical and methyl orange dye. App Catal B-Environ 2012, 123–124: 241–256.View ArticleGoogle Scholar
- Chang BYS, Huang NM, An'amt MN, Marlinda AR, Norazriena Y, Muhamad MR, Harrison I, Lim HN, Chia CH: Facile hydrothermal preparation of titanium dioxide decorated reduced graphene oxide nanocomposite. Int J Nanomedicine 2012, 7: 3379–3387.Google Scholar
- Li YG, Wang HL, Xie LM, Liang YY, Hong GS, Dai HJ: MoS2 nanoparticles grown on graphene: an advanced catalyst for the hydrogen evolution reaction. J Am Chem Soc 2011, 133: 7296–7299. 10.1021/ja201269bView ArticleGoogle Scholar
- Xiang QJ, Yu JG, Jaroniec M: Synergetic effect of MoS2 and graphene as cocatalysts for enhanced photocatalytic H2 production activity of TiO2 nanoparticles. J Am Chem Soc 2012, 134: 6575–6578. 10.1021/ja302846nView ArticleGoogle Scholar
- Kim GP, Nam I, Kim ND, Park J, Park S, Yi J: A synthesis of graphene/Co3O4 thin films for lithium ion battery anodes by coelectrodeposition. Electrochem Commun 2012, 22: 93–96.View ArticleGoogle Scholar
- Wang B, Wang Y, Park J, Ahn H, Wang GX: In situ synthesis of Co3O4/graphene nanocomposite material for lithium-ion batteries and supercapacitors with high capacity and supercapacitance. J Alloy Compd 2011, 509: 7778–7783. 10.1016/j.jallcom.2011.04.152View ArticleGoogle Scholar
- Zhou GM, Wang DW, Li F, Zhang LL, Li N, Wu ZS, Wen L, Lu GQ, Cheng HM: Graphene-wrapped Fe3O4 anode material with improved reversible capacity and cyclic stability for lithium ion batteries. Chem Mater 2010, 22: 5306–5313. 10.1021/cm101532xView ArticleGoogle Scholar
- Lian PC, Zhu XF, Xiang HF, Li Z, Yang WS, Wang HH: Enhanced cycling performance of Fe3O4–graphene nanocomposite as an anode material for lithium-ion batteries. Electrochim Acta 2010, 56: 834–840. 10.1016/j.electacta.2010.09.086View ArticleGoogle Scholar
- Xu K, Ye PD: Theoretical study of atomic layer deposition reaction mechanism and kinetics for aluminum oxide formation at graphene nanoribbon open edges. J Phys Chem C 2010, 114: 10505–10511. 10.1021/jp101387gView ArticleGoogle Scholar
- Park H, Chang S, Jean J, Cheng JJ, Araujo PT, Wang WS, Bawendi MG, Dresselhaus MS, Bulović V, Kong J, Gradečak S: Graphene cathode-based ZnO nanowire hybrid solar cells. Nano Lett 2013, 13: 233–239. 10.1021/nl303920bView ArticleGoogle Scholar
- Zhao MQ, Liu XF, Zhang Q, Tian GL, Huang JQ, Zhu WC, Wei F: Graphene/single-walled carbon nanotube hybrids: one-step catalytic growth and applications for high-rate Li-S batteries. ACS Nano 2012, 6: 10759–10769.Google Scholar
- Kong LY, Ma J, Luan CN, Mi W, Lv Y: Structural and optical properties of heteroepitaxial beta Ga2O3 films grown on MgO (100) substrates. Thin Solid Films 2012, 520: 4270–4274. 10.1016/j.tsf.2012.02.027View ArticleGoogle Scholar
- Gao YH, Bando Y, Sato T, Zhang YF, Gao XQ: Synthesis, Raman scattering and defects of β-Ga2O3 nanorods. Appl Phys Lett 2002, 81: 2267–2269. 10.1063/1.1507835View ArticleGoogle Scholar
- Roy R, Hill VG, Osborn EF: Polymorphism of Ga2O3 and the system Ga2O3-H2O. J Am Chem Soc 1952, 74: 719–722. 10.1021/ja01123a039View ArticleGoogle Scholar
- Ding GQ, Zhu Y, Wang SM, Sun L, Gong Q, Wu TR, Xie XM, Jiang MH: Chemical vapor deposition of graphene on liquid metal catalysts. Carbon 2013, 53: 321–326.View ArticleGoogle Scholar
- Rao R, Rao AM, Xu B, Dong J, Sharma S, Sunkara MK: Blueshifted Raman scattering and its correlation with the  growth direction in gallium oxide nanowires. J Appl Phys 2005, 98: 094312–094315. 10.1063/1.2128044View ArticleGoogle Scholar
- Naumenko D, Snitka V, Snopok B, Arpiainen S, Lipsanen H: Graphene-enhanced Raman imaging of TiO2 nanoparticles. Nanotechnology 2012, 23: 465703–465707. 10.1088/0957-4484/23/46/465703View ArticleGoogle Scholar
- Wu PC, Khoury CG, Kim TH, Yang Y, Losurdo M, Bianco GV, Vo-Dinh T, Brown AS, Everitt HO: Demonstration of surface-enhanced Raman scattering by tunable, plasmonic gallium nanoparticles. J Am Chem Soc 2009, 131: 12032–12033. 10.1021/ja903321zView ArticleGoogle Scholar
- Sidorov AN, Sławiński GW, Jayatissa AH, Zamborini FP, Sumanasekera GU: A surface-enhanced Raman spectroscopy study of thin graphene sheets functionalized with gold and silver nanostructures by seed-mediated growth. Carbon 2012, 50: 699–705. 10.1016/j.carbon.2011.09.030View ArticleGoogle Scholar
- Campion A, Kambhampati P: Surface-enhanced Raman scattering. Chem Soc Rev 1998, 27: 241–250. 10.1039/a827241zView ArticleGoogle Scholar
- Zeng HB, Du XW, Singh SC, Kulin SA, Yang SK, He JP, Cai WP: Nanomaterials via laser ablation/irradiation in liquid: a review. Adv Func Mater 2012, 22: 1333–1353. 10.1002/adfm.201102295View ArticleGoogle Scholar
- Ling X, Zhang J: Interference phenomenon in graphene-enhanced Raman scattering. J Phys Chem C 2011, 115: 2835–2840. 10.1021/jp111502nView ArticleGoogle Scholar
- Kwon KC, Choi KS, Kim SY: Increased work function in few-layer graphene sheets via metal chloride doping. Adv Func Mater 2012, 22: 4724–4731. 10.1002/adfm.201200997View ArticleGoogle Scholar
- Mohamed M, Irmscher K, Janowitz C, Galazka Z, Manzke R, Fornari R: Schottky barrier height of Au on the transparent semiconducting oxide β-Ga2O3. Appl Phys Lett 2012, 101: 132106. 10.1063/1.4755770View ArticleGoogle Scholar
- Xu QJ, Zhang SY: Fabrication and photoluminescence of β-Ga2O3 nanorods. Superlattices Microst 2008, 44: 715–720. 10.1016/j.spmi.2008.09.005View ArticleGoogle Scholar
- Xiao HD, Ma HL, Xue CS, Zhuang HZ, Ma J, Zong FJ, Zhang XJ: Synthesis and structural properties of beta-gallium oxide particles from gallium nitride powder. Mater Chem Phys 2007, 101: 99–102. 10.1016/j.matchemphys.2006.02.021View ArticleGoogle Scholar
- Delpeux S, Beguin F, Benoit R, Erre R, Manolova N, Rashkov I: Fullerene core star-like polymers-1. Preparation from fullerenes and monoazidopolyethers. Eur Polym J 1998, 34: 905–915. 10.1016/S0014-3057(97)00225-5View ArticleGoogle Scholar
- Persson BNJ, Zhao K, Zhang ZY: Chemical contribution to surface-enhanced Raman scattering. Phys View Lett 2006, 96: 207401.View ArticleGoogle Scholar
- McMahon MD, Lopez R, Meyer HM, Feldman LC, Haglund RF: Rapid tarnishing of silver nanoparticles in ambient laboratory air. Appl Phys B Lasers Opt 2005, 80: 915–921. 10.1007/s00340-005-1793-6View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.